# [ACS Symposium Series] New Polymeric Materials Volume 916 || Confined Macromolecules in Polymer Materials and Processes

Post on 11-Dec-2016

215 views

Category:

## Documents

TRANSCRIPT

• Chapter 18

Confined Macromolecules in Polymer Materials and Processes

Peter Cifra* and Tomas Bleha

Polymer Institute, Slovak Academy of Sciences, Dbravsk cesta 9, 842 36 Bratislava, Slovakia

*Corresponding author: cifra@savba.sk

In polymeric systems such as polymer-particle colloid dispersions, composites and nano-composites, clay--intercalates with polymers the geometrical confinement of macromolecules becomes one of crucial features influencing final properties. Confinement is a driving force also in characterization of macromolecules by liquid chromatography (LC). Macromolecular confinement near geometrical obstacle gives rise to a depletion of polymer concentration in the vicinity of wall and to the depletion force. We address the interplay of the confinement, the solvent quality, polymer adsorption, polymer concentration and its consequences for LC and colloid particle-polymer phase behavior. Particularly intriguing is the case of compensation of macromolecular exclusion and adsorption by the confining walls which marks the characteristic inversion of behavior in these fields.

238

Dow

nloa

ded

by T

UFT

S U

NIV

on

Oct

ober

14,

201

4 | ht

tp://p

ubs.ac

s.org

Pu

blic

atio

n D

ate:

Sep

tem

ber 2

9, 2

005

| doi: 1

0.1021

/bk-20

05-091

6.ch01

8

In New Polymeric Materials; Korugic-Karasz, L., et al.; ACS Symposium Series; American Chemical Society: Washington, DC, 2005.

• 239

Introduction

The thermodynamic, conformational and dynamic properties of macromolecular chains are strongly affected by geometrical confinement. This phenomenon is relevant to numerous applications of polymer systems but poses also scientific challenges (i). Polymer chains when confined to a small space exhibit properties distinctly different from those in the unconfined space. Confinement operates also in polymer materials of complex morphology with abundant interfaces which can be approximated by solid walls. There is an important difference between surface/interface and bulk properties of macromolecular chains. Confined flexible polymer chains experience a loss in configuration entropy and this loss can be outweighed by adsorption energy of macromolecules attracted to the surface. The resulting complex behavior poses difficulties to an analytical treatment as well as to experimental studies (2). In this situation molecular simulations become a useful tool (3-6). Simulation can establish a full equilibrium (in contrast to experimental studies often characterized by an incomplete equilibrium and presence of history in adsorptive systems). It can provide local structural information on confined chains and it is possible to deal with perfectly flat surfaces and disregard the surface heterogeneity, surface steps or pre-adsorbed components. Of course, it is possible to study the individual effects either separately or to include the full complexity at later stages.

In this paper we will analyze two examples of confined macromolecular systems which represent general features of phenomena involved in similar systems. First, it is the partitioning of chains into slits, which is underlying the macromolecular characterization and separation by size exclusion chromatography (SEC) and, second, the depletion effects in colloid-polymer dispersions stability. This analysis is accompanied by analysis of concentration profiles including depletion profiles, adsorption profiles and compensation (adsorption vs steric exclusion) profile. The confinement was so far presented mainly through entropie effect (a loss in number of conformations). The effect of confinement, however, varies in the presence of interactions (adsorption, variable solvent quality), chain stiffness, polymer concentration and geometry of confinement or chain architecture. It is the interaction of all these factors which should be well understood.

The partitioning of polymer into porous medium is characterized by the partition coefficient which is the pore(I)-to-bulk(E) concentration ratio at equilibrium, =&. In original theoretical treatment (7) the pure steric exclusion of ideal chains in infinitely dilute solutions was addressed. The analytical approach based on the analogy between diffusion motion of a particle and conformation of a freely-jointed polymer chain provided the relations between the partition coefficient and the coil-to-pore size ratio fc2Rg/D9

Dow

nloa

ded

by T

UFT

S U

NIV

on

Oct

ober

14,

201

4 | ht

tp://p

ubs.ac

s.org

Pu

blic

atio

n D

ate:

Sep

tem

ber 2

9, 2

005

| doi: 1

0.1021

/bk-20

05-091

6.ch01

8

In New Polymeric Materials; Korugic-Karasz, L., et al.; ACS Symposium Series; American Chemical Society: Washington, DC, 2005.

• 240

where Rg is the radius of gyration of a polymer coil and D is the characteristic dimension of a pore. According to theory, the coefficient depends on the confinement ratio only and not on each of these two parameters separately. is related to the free energy of confinement, = -kF \nK, which represents a penalty for the transfer of a molecule from the bulk solution to the solution in pore. Theoretical models of partitioning of flexible macromolecules were recently reviewed (8). The purely steric partitioning of freely-jointed and excluded volume chains into pores with repulsive chain-walls interaction was examined by Monte Carlo (MC) simulations (5-6,9). It was found that partitioning rules for ideal chains according to Casassa (7) have to be modified in the case of excluded volume chains to account for solvent quality and for solute concentration.

The confining porous media in many cases involve pore walls which are attractive to polymer. Polymer partitioning in such cases proceeds via a combined steric exclusion/adsorption mechanism. In order to explain this process the diffusion-equation theory (7) of partitioning of ideal chains was extended (70) to include a short-range segment-wall attraction potential Partitioning of macromolecules in adsorbing pores is examined by theory (10-12) and by simulations (13-14) especially in order to clarify the separation mechanism in LC. The combined effect of purely steric partitioning and wall attraction is particularly noticeable in critical chromatography (15-16) operating close to the critical adsorption strength ^ . Macromolecular solutes adsorb from solution onto a substrate if attractive potential exceeds the critical value & (the adsorption/depletion threshold (7)). At critical condition the entropy loss due to chain confinement into the pore should be compensated by the attractive energy gain and the partition coefficient, K=l, may become independent of the chain length of solute macromolecules (the compensation point). This compensation is used in complex separations, for instance of mixtures including block copolymer. The idea is to find a compensation point for one of the components(blocks) in the mixture. All chain lengths of this component are then moving freely, #=1, between the bulk solution and porous medium, while at the same time the other components are separated according to the chain length. In this way one of the components in LC separation is effectively masked.

Similar confinement situation is characteristic for mixtures of colloid particles and polymers, which are of great practical importance in number of industrial, environmental and medical applications. In general, interaction between polymers and particles can dramatically affect the stability of particle suspensions. The forces between two particles in a solution depend mainly on whether the polymer is attracted (adsorbed) to or repelled (depleted) from the particle surface. An attachment of polymers to the surface, by grafting or by strong adsorption, is a common method of stabilizing large particles in a solution. On the other hand addition of non-adsorbing macromolecules to a

Dow

nloa

ded

by T

UFT

S U

NIV

on

Oct

ober

14,

201

4 | ht

tp://p

ubs.ac

s.org

Pu

blic

atio

n D

ate:

Sep

tem

ber 2

9, 2

005

| doi: 1

0.1021

/bk-20

05-091

6.ch01

8

In New Polymeric Materials; Korugic-Karasz, L., et al.; ACS Symposium Series; American Chemical Society: Washington, DC, 2005.

• 241

colloidal suspension can result in polymer-mediated "depletion attraction" between particle pairs.

The depletion forces in polymer-colloid systems are of a long-standing interest in last few decades. Investigations treated mostly the "colloid limit" where the particle radius Rc greatly exceeds the coil size expressed by the radius of gyration Rg. The depletion mechanism in the colloid limit was first described by Asakura and Oosawa (77). Depletion attraction often leads to demixing into the polymer- and colloid-enriched phases at sufficient polymer concentration. Theoretical and experimental studies on depletion-induced phase separation in colloid-polymer mixtures have recently been reviewed (18). In the colloid limit Rc Rg a colloidal particle resembles a hard planar wall on a relevant length scale. Thus depletion interaction is frequently treated in theory and simulations by a model of a slit formed by two parallel repulsive walls immersed in a polymer solution.

Effect of depletion interaction was so far studied almost exclusively in athermal systems of colloidal particles modeled by hard (repulsive) walls (18, 19). These entropy-driven phase transitions originate solely from the excluded volume interactions. It is of major interest to explore how depletion forces are affected by introduction of a weak attraction potential between polymer and colloidal particles. Inclusion of the energy contribution to the depletion force may assist in portrayal of phase behavior of more realistic colloid-polymer mixtures than are hard particle systems.

Much of the characteristic behavior of confined systems is furnished in concentration profiles at the confining walls. Below we present a general analysis of concentration profiles for the depletion and for the adsorption mode as well as for compensation profile. This is followed by systems with interplay of confinement, polymer-wall and polymer-solvent interactions, variable polymer concentration, together with an illustration of consequences for complex LC separations and colloidal stability. We examine depletion effect and depletion interaction in a weakly attractive slit, particularly in the region around the critical point of adsorption. The method used in Monte Carlo simulation of confined systems has been described in previous paper (20). The simulation of confined polymer chains is performed on a cubic lattice of a lattice unit a with the nearest neighbor non-bonded interactions of segments (in kT units) to account for solvent quality and a similar interaction of polymer segments with the wall to account for the chain attraction to the wall.

Concentration profiles and compensation effect

Depletion profiles. Concentration profiles () shown in Figure 1 depict the situation in the slit represented by hard walls, = 0. Depletion of

Dow

nloa

ded

by T

UFT

S U

NIV

on

Oct

ober

14,

201

4 | ht

tp://p

ubs.ac

s.org

Pu

blic

atio

n D

ate:

Sep

tem

ber 2

9, 2

005

| doi: 1

0.1021

/bk-20

05-091

6.ch01

8

In New Polymeric Materials; Korugic-Karasz, L., et al.; ACS Symposium Series; American Chemical Society: Washington, DC, 2005.

• 242

polymer chains at each wall is seen in all profiles. The concentration profiles are shown in the slit of Dla =12 for chain length = 100 and for the athermal solutions (good solvent) at concentrations (f\ = 0.303, 0.195, 0.120, and 0.032 and for the theta solution at (f\ = 0.286, 0.183, 0.112, and 0.039 in volume fractions. Radius of gyration at infinite dilution and the first overlap concentration for these chains are Rg0= 6.45 (5.34) and ^=0.120 (0.207), for good and theta solvent respectively (9). There is an uneven filling of the space seen in the slit, especially at low concentration. The arrow indicates filling of the space at the walls by increasing concentration. Furthermore, there is another tangible phenomenon that shows a difference between athermal and theta solutions and can be ascribed to the unfavorable segment-solvent interactions. At lower concentrations the two profiles are similar, with a large depletion layer at the slit walls. As the concentration builds up, the athermal chains distribute segments uniformly and are able to fill the depletion layer readily. In the theta solutions, however, the chains do not fill the depletion layer even at high concentrations, but rather build up the concentration in the center region of the slit. Favorable interchain and intrachain interactions allow for this build-up. Alternatively, a lower osmotic pressure in the theta solution in comparison to athermal solution, due to missing second virial coefficient in the theta solvent, is unable to drive the polymer coils into the depletion layer.

Figure 1 Depletion concentration profiles for good solvent (solid lines) and theta solvent (dashed lines). (Reproduced with permission from reference 9.

Copyright 2000 Am. Inst, of Physics)

Dow

nloa

ded

by T

UFT

S U

NIV

on

Oct

ober

14,

201

4 | ht

tp://p

ubs.ac

s.org

Pu

blic

atio

n D

ate:

Sep

tem

ber 2

9, 2

005

| doi: 1

0.1021

/bk-20

05-091

6.ch01

8

In New Polymeric Materials; Korugic-Karasz, L., et al.; ACS Symposium Series; American Chemical Society: Washington, DC, 2005.

• 243

Broader profiles produced by much longer chains in wider slit allow for analysis of the law governing these depletion profiles. Instead of individual profiles as presented above we want to stress universality in these profiles. A reduced plot in terms of the reduced concentration () #,uik as a function of reduced distance / was constructed (27) from simulations of semidilute solutions of athermal chains conducted for JV=2000 (7^=37.7) in the slit of Dla =30, Figure 2. The average density within the slit, reduced by ^ =0.013 was between 4.7 and 8.6 for iV=2000. These concentrations are sufficiently high to allow to estimate the concentration correlation length in the bulk solution by ~ ^goi^uik/^) ^ 3 1 ) , where v/(3v- 1)=0.766. There was a well-defined concentration plateau $,ulk in the density profile in the center section of the slit in each of the simulation results; for these concentrations is expected to be less than 9.25 for = 2000. It means that the effective confinement was weak at these concentrations. At lower concentrations, a plateau in the density profile could not be seen. All the data compiled from different concentrations fall on a single master curve with the correct scaling exponent 1.69 as predicted by scaling theory,$xy$,u\k= (/)1/= (x/)1'69. (For dilute solution this profile scales as ~ (x/Rg)L69.) However, a small shift in distance to the wall by 0.36a had to be introduced. This shift was ascribed to a lattice approximation used in o.i 1 1 ' M 1.69 / / 4.71 - 5.49 / 6.28 7.06 /A /a 8.63 0.1 1 {+0.36) Figure 2 Reduced depletion profile for long chain and five concentrations (Reproducedfrom reference 21. Copyright 2004 ACS) Figure 3 Weak-to-strong penetration transition for good solvent (solid curves) and theta solvent (dashed curves) and series of slit widths D. the simulation (27) but a similar correction was introduced also in analogous off-lattice simulation study (79). Dow nloa ded by T UFT S U NIV on Oct ober 14, 201 4 | ht tp://p ubs.ac s.org Pu blic atio n D ate: Sep tem ber 2 9, 2 005 | doi: 1 0.1021 /bk-20 05-091 6.ch01 8 In New Polymeric Materials; Korugic-Karasz, L., et al.; ACS Symposium Series; American Chemical Society: Washington, DC, 2005. • 244 Increasing the concentration of the polymer in the bulk solution increases the partition coefficient above its value in the dilute limit, Figure 3, and is consistent with the filling of depletion layer by increased concentration, Figure 1. The existence of the weak-to-strong penetration transition was confirmed by simulations (4,9) in slits with repulsive walls and semidilute athermal and theta solutions. The penetration into pores in semidilute solution is governed by the same scaling law as in dilute athermal solutions, only the nature of the entity entering the pore changes from the coil size to a size of concentration blob. The change of solvent quality brings about a qualitative alteration of this behavior in the form of a delayed weak-to-strong penetration transition found on increasing concentration in the theta solvent, Figure 3. Repulsion between chains becomes here effective in pushing the chains into pores at higher concentrations than in good solvents (9) due to missing second virial coefficient. These concentration effects were also studied in solutions of polymer mixtures with the aim to develop an effective technique for separation of macromolecules at higher concentrations and variable solvent quality (22,23). Adsorption profiles. Concentration profiles with polymer adsorption exhibit an enhancement of polymer concentration at the wall in contrast to the depletion profiles. These profiles, however, depend on the adsorption strength of walls towards the polymer chains. First, we concentrate on a strong adsorption of polymer at confining walls. Generally the adsorption profile of macromolecules is, according to de Gennes, divided into several regimes depending on the distance from the surface. From the three typical regimes (proximal, central and distal) for the case of strong adsorption and for semi-dilute concentration the central regime becomes important (24). This is because the proximal range reduces to the monomer size in the limit of strong adsorption and the distal range is effective only in dilute solutions at low adsorption. The universal concentration profile in the central regime is given by the following scaling law, {)/^ = (/?'/)= (x/)'1'299, and for the case of strong adsorption and semidilute solution covers the whole range of profile at the wall. Here d = 3 and =0.588 was used. This scaling was recently verified by simulation (26) for the chain length #=1000 (^=0.0208) and five concentrations in the range of fouiiJf* =1.15-8.41, for which the correlation length granges between 22.92 and 4.99 respectively (compare to i?g(/a=25.52). The chains were athermal representing the good solvent conditions and the adsorption was set to = -1. It is noteworthy that the profile at the wall reaches the correct theoretical slope and the curves for different concentrations are superimposed, Le. form a master curve, Figure 4. Increasing concentration interestingly washes out large differences in adsorption profiles seen between the weak and strong wall attraction (25) in dilute solution. This is seen in partitioning of polymer into attractive pores in Dow nloa ded by T UFT S U NIV on Oct ober 14, 201 4 | ht tp://p ubs.ac s.org Pu blic atio n D ate: Sep tem ber 2 9, 2 005 | doi: 1 0.1021 /bk-20 05-091 6.ch01 8 In New Polymeric Materials; Korugic-Karasz, L., et al.; ACS Symposium Series; American Chemical Society: Washington, DC, 2005. • 245 Figure 5 for chains of #=100 in good solvent. Differences in partitioning seen in the dilute solution for different adsorption strength decrease with concentration and the osmotic pressure induced drive of macromolecules into the pore starts to dominate. The theoretical curves were obtained using Flory (dashed curves) or Huggins (solid curves) relations for the concentration dependence of chemical potential of polymer in partitioning equilibrium between the free and confined solution, ^ = ( - k71n K0, where K0 is the partition coefficient in dilute solution. + KJ+ - \ -+-1.15 - -1 .78 -- A - 2 . 9 4 - -6 .28 --8.41 slope = -1.299\$

. . . . . . . 1 0.1 1

/

Figure 4 Reduced adsorption profiles for long chains and five concentrations. (Reproduced with permission from reference 26. Copyright

2002 MTS) Figure 5 Variation of partitioning with concentration for attractive pores in

good solvent. (Reproduced from reference 25. Copyright 2002 ACS)

Compensation of size exclusion and adsorption. When adsorption strength of the slit walls varies in the range between weak adsorption and strong adsorption, = -1, multitude of concentration profiles appears in which for a certain adsorption strength the characteristic depletion profile turns into the adsorption profile with the opposite curvature. From these many possible concentration profiles we single out three typical situations shown in Figure 6. For a long chain, #=1000, in good solvent at infinite dilution in the slit of width D/a-50 we show a depletion profile (still present for a weak adsorption, = -0.2), an adsorption profile for a stronger adsorption = -0.3 and a typical compensation profile for = -0.2793 with a flat horizontal concentration profile in the wide intra-pore zone except the close proximity to the walls here. The segment concentration is almost independent of the distance from the walls. For perfect compensation the ideally flat concentration profile implies the overall

Dow

nloa

ded

by T

UFT

S U

NIV

on

Oct

ober

14,

201

4 | ht

tp://p

ubs.ac

s.org

Pu

blic

atio

n D

ate:

Sep

tem

ber 2

9, 2

005

| doi: 1

0.1021

/bk-20

05-091

6.ch01

8

In New Polymeric Materials; Korugic-Karasz, L., et al.; ACS Symposium Series; American Chemical Society: Washington, DC, 2005.

• 246

ideal behavior of coils which do not sense the walls as an obstacle. As a result there is a free penetration (K = 1) of coils into pores at the compensation point. This was shown in recent simulation study (14). However, a weak dependence of compensation point on the chain length of polymer was observed which represents a complication in LC separations. Recently a compensation point was estimated not from the compensation condition (K=l) but as a true transition point from the intersection of the partitioning curves (K vs ) for different chain lengths (27). The value ei obtained by this procedure was slightly shifted with respect to the previous method but the weak chain length dependence in partitioning at this critical condition still remained.

Figure 6 Three typical concentration profiles for indicated weak adsorption close to compensation point. (Reproduced from reference 20. Copyright 2004

ACS) Figure 7 Separation modes in liquid chromatography of polymers

In Figure 7 we illustrate three separation modes used in LC, related to three concentration profiles shown in Figure 6, plotted in coordinates employed in this technique. Partitioning coefficient in x-axis is proportional to an elution volume and y-axis to logarithm of molar mass. The standard SEC mode of separation is illustrated by the simulation results on chains (N =100) in good and theta solvent and by respective classical theoretical curve due to Casassa (7) for ideal chains. The adsorption and the compensation mode in LC characterization are shown schematically. The compensation point marking the transition between SEC mode and adsorption mode is sensitive to adjustment conditions as observed also in complex LC studies. This effect is intensively studied (27, 15-16) and is becoming a useful tool for the analysis of complex systems.

Dow

nloa

ded

by T

UFT

S U

NIV

on

Oct

ober

14,

201

4 | ht

tp://p

ubs.ac

s.org

Pu

blic

atio

n D

ate:

Sep

tem

ber 2

9, 2

005

| doi: 1

0.1021

/bk-20

05-091

6.ch01

8

In New Polymeric Materials; Korugic-Karasz, L., et al.; ACS Symposium Series; American Chemical Society: Washington, DC, 2005.

• 247

Depletion interaction in colloidal systems

In addition to already mentioned characteristics of confinement, namely the partition coefficient and the free energy of confinement , the derivative of the free energy d(AA/kT)/aD= -fAT, termed the confinement force, is determined from the simulations of equilibrium of athermal chains in a repulsive slit (6,19,28,29). This force/contributes to the pressure p\ exerted by the confined molecules on the walls inside slit (30, 31). The slit walls also experience a pressure p E from the surrounding bulk solution. The magnitude of the pressures p\ and pE affects the stability of colloidal dispersions. The polymer molecules are excluded from the region near to particle surface (the depletion zone). As the particles approach, the depletion zone minimizes and the coils are pushed out of the gap between the surfaces. The negative value of net pressure ^-. between depletion zones and bulk solution brings about the depletion effect i.e. an effective attraction between colloidal particles. This situation is illustrated in Figure 8.

Figure 8 Depletion interaction between colloid particles at low polymer concentration

The data on the free energy of confinement AA/kT in the dilute solution limit are presented in Figures 9. The term AA represents the free energy of transfer of a macromolecule from a bulk solution of concentration ^ to a solution of concentration $in a slit. The variation of the free energy of confinement AA/kT with the slit width D normalized by the coil diameter 2Rg in the dilute solution limit 0->O is shown for chain lengths JV=100. The curve for =0 corresponds to a purely steric exclusion in a repulsive slit. The confinement penalty AA/kT diminishes by an increase in the attraction strength . The free energy AA/kT is about zero at =-0.2625, close to the critical point of adsorption ^ for this chain length, where the steric exclusion and adsorption effects in the partitioning fully compensate. Perturbation of chains by a presence of the slit walls seems thus fully screened at critical conditions. At the attraction strength higher than the critical one, a molecule in a slit becomes stabilized relative to the bulk phase (AAlkT • 248 DI2R i Figure 9 Free energy of confinement as a function of the reduced slit width for different wall attraction Figure 10 Pressure ratio as a Junction of slit width for different adsorption strength The dot line represents the ideal chain behavior (7). (Reproduced from reference 20. Copyright 2004 ACS) The plot of free energy for purely steric exclusion of athermal chains in Figure 9 resembles the corresponding function for ideal chains (7). The Casassa free energy function of ideal freely-jointed chains confined in a repulsive slit predicts the proportionalities AA~Dl in wide slits and AA~D~2 in narrow slits. The scaling theory (8) that applies only in the limit of narrow repulsive slits suggests the relation AA~D"m for athermal chains. The confinement force calculated from resembles closely the plot of free energy. The force term f/kT is positive at the weak attraction potential and decreases monotonically with increasing separation D. The repulsive nature of the force diminishes by increasing and the force vanishes at the critical point of adsorption. In supercritical region above the force is negative due to adsorption of macromolecules to a single wall or to both walls (particle bridging). In dilute polymer solutions where interchain interactions are negligible the pressure p\ is related to the confinement force / by following relation (30,31) px ^(kTnJV (1 + Df/kT) = idi(l + Df/kT) in which nJVx is the number density of a polymer chain within a slit and nid is the osmotic pressure of ideal solution. In repulsive narrow slits Df/kT 1 and the force term is the leading term. In wide slits or in weakly attractive slits the contribution of the term Df/kT to the pressure p\ becomes insubstantial. The external pressure PE on slit walls in dilute solutions is determined by the osmotic pressure term nl%. Dow nloa ded by T UFT S U NIV on Oct ober 14, 201 4 | ht tp://p ubs.ac s.org Pu blic atio n D ate: Sep tem ber 2 9, 2 005 | doi: 1 0.1021 /bk-20 05-091 6.ch01 8 In New Polymeric Materials; Korugic-Karasz, L., et al.; ACS Symposium Series; American Chemical Society: Washington, DC, 2005. • 249 The above relations lead to the ratio of intra-pore and bulk pressure at full equilibrium in dilute solutions (32) as = (nv\ln%)[\Wf/kT]= K[UDJ7kT]= K+D(dJdD). This equation was employed (32) to compute the ratio pxlpE as a function of the plate separation D under full equilibrium conditions by an analytical theory of solutions of ideal polymers in a repulsive slit. The distinct depletion effect was observed at small separations D. The effect was amplified with an increase in the chain length. Data presented in Figure 9 allow calculating depletion interaction in cases involving non-ideal (excluded volume) chains and weakly attractive slits. The resulting relative pressure pxlpE for chains of #=100 is plotted in Figure 10 as a function of D/2Rg for various attraction strength It is seen that in a repulsive slit (e=0) the intra-slit pressure p\ drops significantly below the bulk pressure pE at the wall separations less than about 3Rg, due to expulsion of molecules from the slit. However, this manifestation of the depletion effect is slightly weaker in excluded-volume chains than in ideal chains. In contrast to force-distance profiles between particles covered by grafted or strongly adsorbed polymers, depletion attraction in systems of non-adsorbing polymers is much smaller and notoriously difficult to measure. Nonetheless, depletion attraction of the type shown in Figure 8 was observed in recent experiments by the AFM technique (33) and the surface force apparatus (34). An increase in the potential substantially reduces the depletion effect, Figure 10; the depletion onset moves to the left below the critical point . By an increase in the mean intra-slit concentration approach the bulk concentration , and the ratio of osmotic pressures (nldi/nldE) converges to unity. As a consequence, the force term Df/kT\m to diminish and finally vanish on increase in in the subcritical region. At critical conditions PilpE-\ in Figure 10; the net pressure ap=0 and the depletion interaction becomes completely ineffective. Above ^ , in the supercritical region, the adsorption layer is formed near the walls and the mean concentration of a polymer in a slit$ exceeds the bulk concentration fe.

The variable p\lpE in Figure 10 can be changed to the relative pressure difference /. An integration of the net pressure hp gives the interaction potential per unit area between the plates W(D) (depletion potential) (17,18). The potential W(D) between two flat walls is related by Derjaguin approximation to the force between two spherical colloidal particles of radius Rc. A knowledge of the effective depletion potential W(D) is a prerequisite of a good understanding of the phase behavior of colloid-polymer mixtures (18). Here we note that at critical condition the depletion potential W(D) vanishes for all plate separations, including the region D/2Rg

• 250

appropriate for ideal chains and repulsive slits. In analogy, the present simulations offer alternative depletion characteristics in situations where polymer-particle attraction potential (or temperature) is used in experiments to regulate (he depletion force and/or the phase behavior.

Depletion effect as described above operates in the dilute solution. It should be noticed, however, that depletion effect builds up with concentration until the coil overlap concentration and then starts to diminish. This can be seen from the confinement force which scales as f/kT ~ ~5/4D 8 / 3 for the semidilute concentration (29).

Conclusions

Confinement of macromolecular systems is traditionally viewed only through the entropy loss. Including interactions of polymer segments with confining walls and with solvent combined with the effect of concentration brings variability with characteristic complex behavior.

Depletion of macromolecules in concentration profiles near the walls diminishes with increasing bulk concentration and varies with solvent quality. Wall attraction in porous medium affects strongly the confinement. At critical attraction the steric exclusion by confinement is compensated by adsorption and this has consequences for instance for complex liquid chromatography separations or for the regulation of stability and phase behavior of polymer-colloid dispersions.

Increased polymer concentration in bulk solution brings a penetration of polymer even into the strong confinement. This penetration transition shifts to higher concentrations for the theta solvents relative to the good solvent and both the shift from the good to the theta solvent and the increased concentration was shown to be interesting for novel complex LC separations.

References

1. Fleer, G.J.; Cohen Stuart, M.A.; Scheutjens, J.M.H.M.; Cosgrove, T.; Vincent, B. Polymers at Interfaces, Chapman & Hall: London, 1993;

2. Frantz, P.J.; Granick, S. Phys. Rev. Lett. 1991, 66, 899-902. 3. Bleha, T.; Cifra, P.; Karasz, F.E. Polymer 1990, 31, 1321-1327 4. Wang, Y.; Teraoka, I. Macromolecules 1997, 30, 8473-8477. 5. Cifra, P.; Bleha, T. Macromolecules 2001, 34, 605-613. 6. Chen, Z.; Escobedo, F.A. Macromolecules 2001, 34, 8802-8810. 7. Casassa, E. F. J. Polym. Sci. Polym. Lett. Ed. 1967, 5, 773-& 8. Teraoka, I. Progr. Polym. Sci. 1996, 21, 89-149

Dow

nloa

ded

by T

UFT

S U

NIV

on

Oct

ober

14,

201

4 | ht

tp://p

ubs.ac

s.org

Pu

blic

atio

n D

ate:

Sep

tem

ber 2

9, 2

005

| doi: 1

0.1021

/bk-20

05-091

6.ch01

8

In New Polymeric Materials; Korugic-Karasz, L., et al.; ACS Symposium Series; American Chemical Society: Washington, DC, 2005.

• 251

9. Cifra, P.; Bleha, T.; Wang, Y.; Teraoka, I. J. Chem. Phys. 2000, 113, 8313-8318

10. Gorbunov, ..; Skvortsov, A. M. Adv. Colloid Interface Sci. 1995, 62, 31-108

11. Guttman, C.M.; DiMarzio, E.A.; Douglas, J.F. Macromolecules 1996, 29, 5723-5733

12. Kosmas, M.K.; Bokaris, E.P.; Georgaka, E.G. Polymer 1998, 39, 4973-4976

13. Davidson, M. G; Suter, U. W.; Deen W. M. Macromolecules 1987, 20, 1141-1146

14. Cifra, P.; Bleha, T. Polymer 2000, 41, 1003-1009 15. Berek, D.; Progr. Polym. Sci. 2000, 25, 873-908 16. Pasch, H.; Trathnigg, B. HPLC of Polymers, Springer-Verlag: Berlin,

1998 17. Asakura, S.; Oosawa, F. J. Chem. Phys. 1954, 22, 1255-&. 18. Tuinier, R.; Rieger, J.; de Kruif, C.G. Adv. Colloid Interface Sci. 2003,

103, 1-31. 19. Milchev, .; Binder, K. Eur. Phys. J. 1998, 3, 477-484. 20. Bleha, T.; Cifra, P. Langmuir, 2004, 20, 764-770 21. Teraoka, I.; Cifra, P. Yongmei Wang Macromolecules 2001, 34, 7121-

7126 22. Wang, Y.; Teraoka, I.; Cifra, P. Macromolecules 2001, 34, 127-133 23. Cifra, P.; Wang, Y.; Teraoka, I. Macromolecules 2002, 35, 1446-1450 24. Daoud M . C. R. Acad. Sci. Paris, Series IV 2000, 1, 1125-1133 25. krinrov, ; Bleha, T.; Cifra P. Macromolecules 2002, 35, 8896-

8905 26. Cifra P. Macromol. Theory Simul. 2003, 12, 270-275 27. Yingchuan Gong; Yongmei Wang Macromolecules 2002, 35, 7492-

7498 28. De Joannis, J; Jimenez, J.; Rajagopalan, R.; Bitsanis, I. Europhys. Lett.

2000, 51, 41-47. 29. Bleha, T.; Cifra, P. Polymer 2003, 44, 3745-3752 30. Vrij, A. Pure Appl. Chem. 1976, 48, 471-&. 31. Clark, A.T.; Lal, M . J. Chem. Soc. Faraday Trans. 2 1981, 77, 981-

996. 32. Ennis, J.; Jnsson, B. J. Phys. Chem. 1999, 103, 2248-2255. 33. Piech, M.; Walz, J.Y. J. Colloid Interface Sci. 2002, 253, 117-129. 34. Ruths, M.; Yoshizawa, H.; Fetters, L.J.; Israelachvili, J.N.

Macromolecules 1996, 29, 7193-7203.

Dow

nloa

ded

by T

UFT

S U

NIV

on

Oct

ober

14,

201

4 | ht

tp://p

ubs.ac

s.org

Pu

blic

atio

n D

ate:

Sep

tem

ber 2

9, 2

005

| doi: 1

0.1021

/bk-20

05-091

6.ch01

8

In New Polymeric Materials; Korugic-Karasz, L., et al.; ACS Symposium Series; American Chemical Society: Washington, DC, 2005.

Chapter 18 Confined Macromolecules in Polymer Materials and ProcessesIntroductionConcentration profiles and compensation effectDepletion interaction in colloidal systemsConclusionsReferences